ANALYSIS OF MORPHOLOGY AND TENSILE STRENGTH OF BANANA
KEPOKFIBRESUSING A SCANNING ELECTRON MICROGRAPH
(SEM) AND PULL TEST EQUIPMENT
Atus Buku and G. N. Anastasia Sahari
Departement of Mechanical Engineering, Paulus Christian University of Indonesia, Makassar, Indonesia E-Mail: email@example.com
Banana plants are plants typical of tropical regions which can be easily found anywhere without knowing the season. Until now the use of banana plants in Indonesia has been merely the cultivation of fruit and there is very little use of other parts of this banana tree.The purpose of this study was to uncover behavioural engagement capability and Interfacial shear stress banana fibres cured epoxy matrix due to the soaking treatment of alcohol. Alcohol soaking treatment banana kapok fibre variation alcohol content of 0%, 70%, and 95%, and the soaking time of 8 hours.Banana fibre without and with soaking treatment was observed by SEM to determine the ability of the engagement fibre with epoxy matrix and also for banana fibre surface morphology. Tensile test was conducted to determine the interfacial shear strength by embedding a single fibre banana fibre into the epoxy matrix as deep as 1 mm. The test results showed that the soaking treatment causes the fibre surface becomes coarse, wrinkled, uneven forming grooves in a longitudinal direction and transverse impact on improving the ability of the engagement between banana fibre with epoxy matrix. Shear stress epoxy
matrix interface with banana fibre without soaking treatment of alcohol obtained 2,358 kgf / mm2, at 70% alcohol
immersion shear stress 1.542 kgf / mm2 and at the 70% alcohol immersion shear stress 1,254 kgf / mm2.
Keywords: morphology, tensile strength, fibre, banana kepok, scanning electron micrograph (SEM), pull test equipment.
Banana plants are plants typical of tropical regions which can be easily found anywhere without knowing the season. Until now the use of banana plants in Indonesia has been merely the cultivation of fruit and there is very little use of other parts of this banana tree. The addition of natural fibres into the composite is expected to improve the mechanical properties, namely tensile and
flexural strength of the composites (Ibrahim et al., 2010;
Rozman et al., 1998; Nair et al., 1996).
Singh et al. (2012) conducted research on
bananas and powdered silica fibre reinforced composite materials are developed, the results of this study were obtained scanning electron microscopy showed that the banana fibres are well dispersed in the matrix resin.The addition of banana fibres greatly reduces the yield strength and the addition of silica gives better results from banana fibre reinforced composites but still has a yield strength is greatly reduced. Natural rubber composite lamina reinforced with banana stem fibres by a mixture of NaOH and Na2SO3 has superior tensile strength (Sahari et al., 2015).While the tensile strength, flexural strength, impact strength in woven banana pseudo stem Increased reinforced epoxy composites. Banana fibre composites showed a resilient performance with minimum plastic
deformation (Maleque et al., 2011; Pothan et al., 2009;
Magdaet al., 2010; Wuryanti, 2013). Giving coagulum in
the polyester fibre banana can increase of the composite index, limiting oxygen from 18 to 21% with a reduction in
smoke density (Budinsky et al., 2003; Thiruchitrambalam
2011; Maleque et al, 2008; Mukhopadhyay etal, 2008).
Banana fibre in combination with an excellent glass to
create a low cost composite materials (Pothan et al.,
Based on the brief description above, the research of natural fibres, especially cellulose fibre banana cured by soaking treatment by using a variable amount of alcohol.A series of tests to uncover the effect of submergence of alcohol on the fibre surface morphology and the ability of the engagement interface with fibre epoxy matrix and shear strength fibre with an epoxy matrix with the test method pull out.
MATERIALS AND METHODS
Materials used consist of:
Banana kapok fibre with an average age of 10 months,
with a leaf length of about one meter, then soaking for 2 weeks to rot. Furthermore, the fibre is separated from the skin leaves have decomposed, then cleaned with distilled water to clean dirt and then dried at room temperature 31 °C. Furthermore, alcohol soaking treatment is done with alcohol composition 70 and 95% of soaking for 10 hours.
Composites, a composite material are used as a
damage due to collision impact. Generally the matrix material can include metals, polymers, ceramics,
carbon (Reddy et al., 2014). While the fibre material
that is commonly used is carbon fibre, glass fibre, ceramics. However, lately the natural fibres are already Began ogled as an alternative eco-friendly fibre. Two important terms in the composite namely Lamina and Laminate. Based on the placement there are several types of fibre in composites, namely: (1) Continuous Fibre Composite; (2) Woven Fibre Composite (bi-directional); (3) discontinuous Fibre Composite and (4) Hybrid Fibre Composite. Discontinuous FibreComposite is the type of composites with short fibres. This type is
distinguished into three, namely: Aligned
discontinuous fibre, Off-axis aligned discontinuous fibre and Randomly oriented discontinuous fibre.
Resin, generally resin is the material to be reinforced
with fibres. Resin is a low viscosity liquid, which hardens after the polymerization process. Serves as a binder resin (bounding) between the fibres to one another so as to produce a strong bond formed solid composite material, which is a material that has the bond strength is high (Budinski, 2003). The resin is used in most Thermosetting, b). Phenolic, c).Epoxy and polyester. Plastic waste classified as polyester resin/thermoplastic that has the characteristics of resistance to strong acids except oxidizing acid, but
weak against alkali (Monteiro et al., 2008; Surdia,
1989; Smith, 1999 and Shackelford, 1996). Polyester resin is the most widely used as a matrix for fibre glass hull, automobile, water tanks and so forth
(Naveen et al., 2012).
Catalyst, a catalyst is used to assist the drying process
of resin and fibres in the composite. The time needed to transform into a plastic resin depends on the
amount of catalyst is mixed (Chorkendorff et al,
2007; Sheldon et al., 2007). The addition of a good
catalyst 1% of the volume of resin. If there is a reaction will occur between 60-90°C heat. This heat is sufficient to react the resin in order to obtain the strength and form of plastic that maximum inaccordance with the desired shape of the mold
(Deutschmann et al., 2009; Schuit et al., 1973)
Testing Scanning Electron Micrograph (SEM)
SEM is a tool that can form the image of the specimen surface microscopically. The electron beam with a diameter of 5-10 NM is directed at the specimen. The interaction of the electron beam with the specimen produce some phenomena items, namely backscattering electron beam, x-rays, secondary electrons and electron
absorption (Abed et al., Stadtlander, 2007). SEM
technique is the investigation and analysis of surface.
The tensile test is used to determine the tensile strength of a specimen.
Table-1. Specifications tools.
Capacity Kg 20,000
Units Load N,kN,g,kg,ton,ib
Load Resolution 1/20000
Load Accuracy ±1% (0,5% optional)
Load Amplification x1,x2,x5,x10 Auto range
Test width (mm) 575
Crosshead Travel (mm) 1440
Testing stroke Crosshead travel minus upper/lower grips and gauge length
Range of test speed (mm/min) 0.2-, 200
Max, load at full speed (kgf) 2000
Max. speed at full load (mm/min) 50
Speed Accuracy ±0.5% servo control
Resolution (mm) 0,001
Driving Motor AC Servo Motor
Power 3Ø22VAC,50/60Hz (380/415V optional)
Dimensions (cm) 125x90x280
the standard used:
Tensile test carried out by using the standard American Society For Testing and Materials (ASTM). Wherein the dimensions of the specimen as shown in the figure below:
Figure-2. Tensile test specimens.
Wo = the notch width 25 mm;
A = sectional area of 120 mm ;
L = long specimen 150 mm;
Lo = long notch 80 mm ;
h = thick specimen 8 mm.
Fibre morphology test
(a) non alcohol (b) alcohol 70% (c) alcohol 95 %
Figure-3. Banana Kepok fibres were soaked for 8 days.
(a) non alcohol
(b) alcohol 70% (c) alcohol 95%
2 4 6 8 10 12 14 16 18 20
keV 0 2 4 6 8 10 12 cps/eV
Al Si Na Mg
Ti O P S S
2 4 6 8 10 12 14 16 18 20
keV 0 2 4 6 8 10 12 14 16 cps/eV
Na Mg K
Si P S S O
2 4 6 8 10 12 14 16 18 20
keV 0 2 4 6 8 10 12 cps/eV
Na Mg K
Ca O Al
Si P S S
Figure-5. Banana kepok fibre composition test results the treated.
The longer the soaking fibre by using alcohol would result in the decrease in calcium, potassium in fibre. Reduction of calcium affects the fragility of these fibres. The function of potassium in plants is a catalyst that is highly active nutrients. Average tensile strength fibre composite with untreated slightly lower than the composite fibres treated with alcohol.This happens due to small differences in percentage and percentage of alcohol used in this study, so that almost no significant difference in tensile strength. Treatment of alcohol on the fibre causes partial loss of hemicellulose, lignin, wax and other impurities on the surface of the fibre.Surface topography becomes coarser fibres resulting mechanical interlocking. With the loss of lignin and various other impurities in the fibre surface, the field of chemical reactions and bonding between the fibres and the matrix increases the mechanical properties. Because in this study, the percentage used is too large, so much influence on the fibre surface conditions. This is shown in the fracture topography of the specimen is also quite similar (Figure-4).
Based on Table-2 shows that the tensile strength of the composite is soaked in alcohol is lower than without soaking alcohol. Topographic cross-section of the fault (Figure-4) it seems that the more alcohol without soaking the fibre pullout compared with alcohol immersion. This shows that with no alcohol soaking, the water more easily gets into polyester and eventually absorbed by the fibre so that the bonding surface with a matrix fibres (polyester) experienced depending and eventual release of the ligament fibre and polyester. The longer soaking the alcohol molecules are absorbed by the fibre resulted in fibre swell. Liberation bonding with polyester fibre surface and also the dissemination of fibre resulting in mechanical damage or damage to the mechanical strength of the composite, as shown in Figure-3 SEM cross section. the composition of the high alcohol content result in damage to the structure of the fibre. This damage affects the fragility of fibre.
Table-2. Results of pull testing composite fibre Banana kepok.
Alcohol levels P σ ΔL ε E
(kgf) (kgf/mm²) (mm) X100 % % (kgf/mm²)
Non-alcohol 283 2.358 2,358 0.029 2.9 81.31
70 % 185 1.542 1,542 0.019 1.9 81.158
(Figure-4). From Table-2 shows that the tensile strength composite without soaking alcohol is higher than the soaked with alcohol.
From the test results can be concluded that banana fibres are not soaking alcohol has a higher tensile
strength than the through immersion alcohol. The fibre is
through immersion with the percentage of alcohol that are too large can result in fevers become brittle. The fragility of the fibre due to the release of fibres with polyester bonding surface and also delamination in fibre resulting in mechanical damage or deterioration of the mechanical strength of the composite.
Abed S. A., Ibnsouda S. K., Latrache H. and Hamadi F. 2007. Scanning Electron Microscopy (SEM) and Environmental SEM: Suitable Tools for Study of
Adhesion Stage and Biofilm Formation.
www.intechopen.com. pp. 717-730.
Budinski K. G. 2003. Engineering Material Properties and Selection. New Jesey : Prentice Hall.
Chorkendorff, I. and Niemantsverdriet J. W.
2007.Concepts of Modern Catalysis and Kinetics, Second Edition.WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, Germany.
Deutschmann O., Ozinger H., Kochloefl K. and Turek K. 2009. Heterogeneous Catalysis and Solid Catalysts, WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, Germany.
Ibrahim M. M., Dufresne A., El-Zawawy W. K. and Agblevor F., A. 2010. Banana ﬁbers and Microﬁbrils as Lignocellulosic Reinforcements in Polymer Composites. Carbohydrate Polymers, 81:811–819.
Magda G. E., Mohamed S. H. and Mahani, R. M., 2010. Study Mechanical, Swelling and Dielectric Properties of Prehydrolysed Banana ﬁber- Waste Polyurethane Foam Composites. Carbohydrate Polymers. 80: 366-372.
Maleque, A. M., Saiful, A. and Sapuan, S. M. 2005. Effect of Volume Fraction of Pseudo-Stem Banana Fiber on the Properties of Epoxy Composite, International Conference on Mechanical Engineering 2005.
Maleque A. M. and Belal F. Y. 2009. Mechanical Properties Study Of Pseudo-Stem Banana Fiber Reinforced Epoxy Composite.The Arabian Journal for Science and Engineering. 32:2B.
Mukhopadhyay S., Fangueiro R., Arpaç Y.and Şentürk Ü.
Nair M., Diwan S. M. and Sabu S. 1996.Journal Applied Polimer Science.
Naveen P. N. E. and Raju T. D. 2012. Evaluation of Mechanical Properties of Coir Fiber Reinforced Polyester Matrix Composites. International Journal of Mechanical and Industrial Engineering (IJMIE). 2(4):2231-6477.
Pothan A. L. and George N. C. 2009.Dynamic Mechanical and Dielectric Behavior of Banana-Glass Hybrid Fiber Reinforced Polyester Composites. Journal of Reinforced Plastics and Composites. 29(8):1131-1145.
Pothan A. L., Thomas S. and George J. 2010. Tensile and Impact Properties of Banana Fibre/Glass Fibre Hybrid Polyester Composites. Journal of Reinforced Plastics and Composites. 29: 1131-1145.
Radzi M. H. A. and Saleh M. A. N. 2011. Banana Fiber Reinforced Polymer Composites. Empowering Science, Technology and Innovation towards a Better Tomorrow.
Raghavendra S.,Lingaraju, Shetty P. B. and Mukunda P. G. 2013. Mechanical Properties of Short Banana Fiber Reinforced Natural Rubber Composites. International Journal of Innovative Research in Science, Engineering and Technology. 2(5):1652-1655.
Reddy M. I. and Reddy V. S. 2014. Dynamic Mechanical Analysis of Hemp Fiber Reinforced Polymer Matrix Composites. International Journal of Engineering Research & Technology (IJERT). 3(9):410-415.
Rozman H. D., Kon B. K., Abu S., Kumar R. N. and Ishak
M. 1998. Rubberwood-High-Density Polyethylene
Composites: Effect of Filler Size and Coupling Agents on Mechanical Properties. Journal Applied PolimerScince. 69(10): 1993-2004.
Sahari G. N. A. and Buku A. 2015. Tensile Strength of Fiber for Some Type Bananas (Ambon, Kepok, Susu). IJRET: International Journal of Research in Engineering and Technology. 04(08): 183-186.
Schuit G. C. A. and Gates B. C. 1973. Chemistry and Engineering of Catalytic Hydrodesulfurizition.Journal Review. 19(3): 417-438
Sheldon R. A., Arends I. and Hanefeld U. 2007.Green Chemistry and Catalysis, WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim, Germany.
Singh V. K., Gope P. C., Sakshi C. and Singh B. D. 2012.Mechanical Behavior of Banana Fiber Based Hybrid Bio Composites. Journal Mater. Environ. Sci.3:185-194.
Shackelford J. F. 1996. The mechanical properties composite, Acta. Metall. Mater. 40:177-184.
Smith W. F. 1999. Principles of Material Science and Engineering. New York: Mc.Granhill Book Company.
Thiruchitrambalam M., Alavudeen A., Athijayamani A., Venkateshwaran N., Perumal E. 2009. Improving Mechanical Properties of Banana/Kenaf Polyester Hybrid Composites Using Sodium Laulryl Sulfate Treatment. Materials Physics and Mechanics. 8:165-173.
Twite M., Kovaleva E., Munyaneza J. and Habimana V. 2011. Assessment of Natural Adhesives in Banana Leaf Composite Materials for Architectural Applications. Second International Conference on Advances in Engineering and Technology.